- Nano Express
- Open Access
Dual Functions of V/SiOx/AlOy/p++Si Device as Selector and Memory
Nanoscale Research Letters volume 13, Article number: 252 (2018)
This letter presents dual functions including selector and memory switching in a V/SiOx/AlOy/p++Si resistive memory device by simply controlling compliance current limit (CCL). Unidirectional threshold switching is observed after a positive forming with low CCL of 1 μA. The shifts to the V-electrode side of the oxygen form the VOx layer, where the threshold switching can be explained by the metal-insulation-transition phenomenon. For higher CCL (30 μA) applied to the device, a bipolar memory switching is obtained, which is attributed to formation and rupture of the conducting filament in SiOy layer. 1.5-nm-thick AlOy layer with high thermal conductivity plays an important role in lowering the off-current for memory and threshold switching. Through the temperature dependence, high-energy barrier (0.463 eV) in the LRS is confirmed, which can cause nonlinearity in a low-resistance state. The smaller the CCL, the higher the nonlinearity, which provides a larger array size in the cross-point array. The coexistence of memory and threshold switching in accordance with the CCL provides the flexibility to control the device for its intended use.
Resistive random-access memory (RRAM) is one of the promising candidates for the next-generation non-volatile memory technology due to its fast switching speed [1, 2], low-power consumption [3,4,5,6,7,8], multilevel capability [9,10,11,12,13,14,15], high scalability [16,17,18,19,20], and 3D stacking ability [21,22,23,24,25]. These properties are especially suitable for storage class memory (SCM) which can fill the performance gap between dynamic random-access memory (DRAM) as a main memory and solid-state-drive (SSD) as a storage memory. Even though RRAM device has made much progress in the past years [1,2,3,4,5,6,7,8,9,10,11,12,13,14,15,16,17,18,19,20,21,22,23,24,25], there remains, however, a major disadvantage: sneak current through neighboring cells occurs in a high-density cross-point array . The memory device with the selector component should provide nonlinear current–voltage (I–V) characteristics to overcome this problem [26,27,28,29,30,31,32,33,34,35]. Until now, various devices with nonlinear concepts such as complementary resistive switching (CRS) , tunnel barrier [27,28,29,30,31,32,33], Ag-based threshold switching , diode-type selector [35, 36], ovonic threshold switching (OTS) [37, 38], and metal-insulator-transition (MIT) [39,40,41,42,43] have been reported. VOx as one of the typical MIT materials could be widely used in potential applications as optical and electrical switching component [40,41,42]. SiO2 is widely used as a passivation layer in the semiconductor industry. Moreover, Si-rich SiOx (x < 2) can be used as a resistance change layer in RRAM [44,45,46,47,48,49,50,51,52,53,54,55]. SiOx can be preferred over many other materials in terms of compatibility with CMOS processes and low cost. SiOx-based RRAM devices have been reported to act as a mediator of the role of conducting bridges simply by using electrodes such as Cu and Ag with high diffusivity [44,45,46,47]. In another case, memory switching is induced by the valence change effect inside the SiOx layer, which can be explained by generation of oxygen vacancies or proton exchange model [48,49,50,51,52,53,54,55]. In the unipolar switching where a set operation precedes a reset, it is sensitive to the ambient atmosphere. The switching performance in the air is significantly degraded [48,49,50,51,52,53]. On the other hand, filamentary switching without backward-scan effects shows typical unipolar and bipolar switching in various SiOx-based RRAM devices [52,53,54].
Here, we present the coexistence of threshold switching and memory switching in V/SiOx/AlOy/p++Si device depending on compliance current limit (CCL). The device with silicon bottom electrode (BE) has several advantages compared to the conventional metal electrode. The RRAM device with memory or threshold switching is directly connected to the source or drain side in a transistor, which is a potential application for embedded memory and steep slope device. The overshoot current could be reduced due to the series resistance of Si BE. Moreover, nano-tip of silicon BE through wet etching and the adjustment of the doping concentration in silicon surface can improve switching performance. The AlOy layer, which is a large band gap with an insulated property, helps to lower the operating current during threshold and memory switching. The SiOx layer acts as memory switching layer at a high CCL, while it serves to supply oxygen to V TE at low CCL, which provides threshold switching.
V/SiOx/AlOy/p++Si device was fabricated as follows: Firstly, BF2 ions were implanted with an acceleration energy of 40 keV and a dose of 5 × 1015 cm−2 into a Si substrate to heavily doped Si BE. The lattice damage was cured by the annealing process at 1050 °C for 10 min. Heavily doped Si BE had sheet resistance of 30.4 Ω/□. Next, a 1.5-nm-thick AlOy layer was deposited by an atomic layer deposition (ALD) system using H2O and Al (CH3)3 and a 5.5-nm-thick SiOx layer underwent plasma-enhanced chemical vapor deposition (PECVD) by reacting 5% SiH4/N2 (160 sccm), N2O (1300 sccm), and N2 (240 sccm) at 300 °C. Subsequently, a 50-nm-thick vanadium (V) top electrode (TE) with a diameter of 100 μm was deposited by DC sputtering a V target with Ar gas (30 sccm). Finally, a 50-nm-thick Al as a protective layer was deposited by DC sputtering to prevent further oxidation of V TE. All electrical properties were characterized via the DC voltage sweep and pulse modes using a Keithley 4200-SCS semiconductor parameter analyzer (SPA) and a 4225-PMU ultra-fast current–voltage (I–V) module at room temperature, respectively. For device operation, the TiN BE was grounded and the Ni TE bias was controlled.
Results and Discussion
Figure 1a shows the schematic structure of V/SiOx/AlOy/p++Si device. Three amorphous V, SiOx, and AlOy layers and single-crystalline Si layer are observed by a transmission electron microscopy (TEM) cross-sectional image as shown in Fig. 1b. The thicknesses of the SiOx and AlOy layers are 5.5 and 1.5 nm, respectively. To confirm the composition ratio of two dielectric films, XPS analysis was conducted (Additional file 1). The x value of SiOx and the y value of AlOy are 0.88 and 1.33, respectively. Our SiOx film using PECVD compared to SiO2 deposited using dry oxidation is deposited at a much lower temperature and has much more defects, making them suitable for resistive switching at relatively lower voltages. Figure 2a shows typical threshold switching of V/SiOx/AlOy/p++Si device. The initial switching with a positive forming process requires higher voltage than subsequent threshold switching since the dielectric layers have initially smaller defects. A CCL of 1 μA is applied to the device to avoid the formation of excessive conducting filaments in the SiOx layer. The leakage current is very low (100 pA at 1 V) compared with previously reported threshold switching of VOx. This advantage is attributed to the Al2O3 with higher permittivity and thermal conductivity compared to the SiO2. Off-state has the insulating property because the filaments are easily ruptured and then there are no remaining filaments. A possible mechanism for threshold switching is the oxidation of the V TE from the oxygen supplied from the SiOx layer during the positive forming process as shown in Fig. 2b. The electrical property of VOx between V TE and SiOx layer may change from insulating state to metallic state, causing a sudden change in resistance. A low CCL of 1 μA is not sufficient to cause efficient conducting filaments inside the SiOx film. Therefore, SiOx with insulating properties can be another cause to reduce the off-current. For a negative forming process of V/SiOx/AlOy/p++Si device, a threshold switching is not observed (see Additional file 1). When the negative bias is applied to the V TE, the movement of the oxide moves toward the Si BE, so that the V TE can no longer participate in the threshold switching as VOx. Inset of Fig. 2a exhibits the threshold voltage (Vth) and hold voltage (Vhold) during the 100 cycles. The Vth where the current sharply increases with nearly infinite slope is between 1.08 and 1.82 V, and Vhold at which point the current return to a high-resistance state is between 0.12 and 0.54 V. Figure 2c shows the I–V characteristics in the on-current at different temperatures. At 25 °C and 55 °C, they show almost similar threshold switching, but I–V curve at a higher temperature of 85 °C loses the threshold switching property. It is well known that VOx loses its MIT at high temperatures. Thus, this result is another proof that VOx is the main cause of the threshold switching. Figure 2d shows the transient characteristics for threshold switching. The pulse with the amplitude of 1 V monitored the read current before and after writing pulse with width of 1 μs. The high current was monitored while the pulse with high amplitude is applied to the device, and then, the V/SiOx/AlOy/p++Si device turned off the current immediately after the writing pulse was removed. The selector properties analyzed above can be used when combined with operation of memory elements below 1 μA [55, 56].
Figure 3a shows the bipolar resistive switching of V/SiOx/AlOy/p++Si device after a positive forming with CCL of 100 μA. Then, the reset process with a rapid increase in resistance is performed by sweeping the negative voltage, and the device is switched to a high-resistance state (HRS). The set process with a rapid decrease in resistance then occurs at a positive bias voltage, causing the device to turn back to a low-resistance state (LRS). In order to understand the properties of the conducting filament, we observe the normalized conductance and the temperature dependence. The conduction in the LRS is an important guideline to indirectly inform the properties of the conducting filament. Figure 3b shows the normalized conductance (GN) which is defined as the dynamic conductance (Gd) divide by static conductance (G0) for I–V curves of V/SiOx/AlOy/p++Si device in the LRS with different temperatures. Regardless of the temperature, the GN value converges to 1 when the voltage is zero. This allows us to rule out the well-known conduction mechanism such as Schottky emission, Fowler-Nordheim tunneling, and Child’s law (I~V2) in space-charge-limited current (SCLC). Metallic ohmic conduction can also be excluded considering temperature dependence as shown in Fig. 3c. The decrease in resistance with increasing the temperature suggests that the conducting filament has a semiconducting property. Thus, we can exclude the penetration of V into the SiOx layer for the main conducting filament of V/SiOx/AlOy/p++Si device in LRS. Therefore, the bipolar memory operation of the V/SiOx/AlOy/p++Si device is dominated by intrinsic switching of SiOx. It is also confirmed that the positive and negative currents are not that much different suggesting that rather than an interface-type such as Schottky emission, it is dominated by bulk conduction. Taking into account the abovementioned normalized conductance, there are two possible bulk dominant conduction mechanisms. The first one is hopping conduction following the formula:
where q, n, a, øT, vo, and d are the electric charge, concentration of space charge, mean of hopping distance, electron barrier height for hopping, intrinsic vibration frequency, and the thickness of dielectric film, respectively. The øT calculated from the slope of a linear plot of ln (I) versus 1000/T is 0.463 eV as shown in Fig. 3c. A value calculated from the relationship between Ea and V is 5.17 nm, indicating the conducting filament formed in the SiOx is not strong and is close to the HRS state. The other conduction mechanism, the Poole-Frenkel (P-F) emission, was covered in Additional file 1. Based on the above results, the conducting filament model in the memory operation of V/SiOx/AlOy/p++Si device is depicted in Fig. 3d. In the positive forming process, the oxidation process proceeded on the V TE side, but due to the high CCL, a conductive filament can be formed inside the SiOx and AlOy due to the movement of the oxygen vacancies. During the reset process, the electric field opposite to the forming and set induces oxygen and recombination with the oxygen vacancy, resulting in the rupture of the conductive filament. It is noted that the selector and memory operations are observed in the same cell. Memory operation is possible after the threshold operation has occurred and then the switch is completely turned off. However, the reverse direction is not possible because the reset switching of the memory operation is not completely turned off.
Figure 4a shows normalized I–V curves in the LRS of V/SiOx/AlOy/p++Si device at low-voltage regime (0~1 V) for different CCL conditions (5 μA, 30 μA, and 1 mA). Here, the normalized I–V curve is defined as the current at each voltage divided by the current at 1 V. Since the levels of the LRS current depending on the CCL are varied, we set the current value at 1 V to easily compare the nonlinearity. It can be observed that as the CCL decreases, the current is suppressed at lower voltage regime. In order to derive a more quantitative relation, nonlinearity is defined as the ratio of the current at VREAD to that at the half of VREAD. Figure 4b shows the read current at 1 V and nonlinearity as a function of CCL for V/SiOx/AlOy/p++Si device. The decrease in read current due to CCL reduction suggests that the conducting filament is becoming finer and then the nonlinearity increases. The intrinsic silicon oxide film exhibits high nonlinearity even in a single layer. The intrinsic nonlinear property is due to the bulk nature of the silicon oxide rather than the interface of the silicon. The smaller the CCL is, the less the degradation is generated in the SiOx, so the lowering of the trap energy level in the LRS compared to that in the HRS can be minimized. Therefore, the higher energy barrier can maximize nonlinearity in the LRS state when lower CCL is applied to the device. Similarly, the conduction described by the P-F emission in the TaOx/TiOy stack ensures high nonlinearity . Another possibility is that because the dielectric constant of the oxide is smaller, more passes are made to the oxide film due to the concentration of the field. This can lead to the lowering of the trap energy level of the oxide layer, which can be expected to serve as a tunnel barrier for Al2O3. To obtain to the read margin (∆V) in n × n cross-point array, we use the simplified equivalent circuit as shown in Fig. 4c. Considering the worst case, the adjacent cells are set to the LRS and the load resistance (RL) to the LRS resistance. The ∆V was calculated from difference between VOUT at LRS and VOUT at HRS. Figure 4d shows the ∆V as a function of number of word lines (n) for V/SiOx/AlOy/p++Si device. The smaller the CCL, the higher the ∆V because the nonlinearity increases. When 10% read margin is secured, the array can be expanded to about more than 10 × 10 for CCL of 5 μA and to 5 × 5 for CCL of 1 mA. The array size to withstand the sneak current is not sufficient, but it will help expand the array size when the device with selector function is connected in a V/SiOx/AlOy/p++Si device. Compared to 0.5-V read in all CCLs, it has higher nonlinearity with read at 1 V. Although low VREAD leads to low static power in the read operation, the value of nonlinearity becomes smaller, which is due to the fact that the electric field is less on the SiOx/AlOy layer in smaller VREAD.
In this work, a V/SiOx/AlOy/p++Si device having both a selector and a memory function by simply controlling CCL is investigated. When a CCL of 1 μA or less is applied, unidirectional threshold switching is observed for selector application. Positive forming oxidizes the V electrode and the MIT phenomenon of VOx can induce threshold switching. The AlOy layer is able to achieve a high selectivity of 104 by lowering the off-current. On the other hand, when a CCL of 5 μA or more is applied, memory switching is observed as effective conducting filaments are formed on the SiOx layer. The lower the CCL, the greater the nonlinearity, which helps to increase the size of the cross-point array.
Atomic layer deposition
Compliance current limit
Complementary resistive switching
Dynamic random-access memory
Ovonic threshold switching
Plasma-enhanced chemical vapor deposition
Resistive random-access memory
Storage class memory
Semiconductor parameter analyzer
Transmission electron microscopy
Lee MJ, Lee CB, Lee D, Lee SR, Chang M, Hur JH et al (2011) A fast, high endurance and scalable non-volatile memory device made from asymmetric Ta2O5-x/TaO2-x bilayer structures. Nat Mat 10:625–630
Luo W-C, Liu J-C, Feng H-T, Lin Y-C, Huang J-J, Lin K-L et al (2012) RRAM set speed-disturb dilemma and rapid statistical prediction methodology. IEEE Int Electron Devices Meet Tech Dig 9:5.1–5.4
Kim S, Chang YF, Kim M-H, Bang S, Kim TH, Chen YC, Lee J-H, Park B-G (2017) Ultralow power switching in silicon-rich SiNy/SiNx double-layer resistive memory device. Phys Chem Chem Phys 29:18988–18995
Ye C, Zhan C, Tsai TM, Chang KC, Chen MC, Chang TC et al (2014) Low-power bipolar resistive switching TiN/HfO2/ITO memory with self-compliance current phenomenon. Appl Phys Express 7:034101
Kim S, Jung S, Kim MH, Cho S, Park BG (2015) Resistive switching characteristics of Si3N4-based resistive-switching random-access memory cell with tunnel barrier for high density integration and low-power applications. Appl Phys Lett 106:212106
Banerjee W, Rahaman SZ, Prakash A, Maikap S (2011) High-κ Al2O3/WOx bilayer dielectrics for low-power resistive switching memory applications. Jpn J Appl Phys 50:10PH01
Wu Y, Yu S, Lee B, Wong P (2011) Low-power TiN/Al2O3/Pt resistive switching device with sub-20 μA switching current and gradual resistance modulation. J Appl Phys 110:094104
Wu M-C, Lin Y-W, Jang W-Y, Lin C-H, Tseng T-Y (2011) Low-power and highly reliable multilevel operation in ZrO2 1T1R RRAM. IEEE Electron Device Lett 32:1026–1028
Hsu CH, Fan YS, Liu PT (2013) Multilevel resistive switching memory with amorphous InGaZnO-based thin film. Appl Phys Lett 102:062905
Liu M, Abid Z, Wang W, He XL, Liu Q, Guan WH (2009) Multilevel resistive switching with ionic and metallic filaments. Appl Phys Lett 94:233106
Abbas Y, Jeon YR, Sokolov AS, Kim S, Ku B, Choi C (2018) Compliance-free, digital SET and analog RESET synaptic characteristics of sub-tantalum oxide based neuromorphic device. Sci Rep 8:1228
Long S, Perniola L, Cagli C, Buckley J, Lian X, Miranda E, Pan F, Liu M, Suñé J (2013) Voltage and power-controlled regimes in the progressive unipolar RESET transition of HfO2-based RRAM. Sci Rep 3:2929
Kim MH, Kim S, Bang S, Kim TH, Lee DK, Cho S, Lee JH, Park BG (2017) Pulse area dependent gradual resistance switching characteristics of CMOS compatible SiNx-based resistive memory. Solid State Electron 132:109–114
Kim S, Park BG (2016) Nonlinear and multilevel resistive switching memory in Ni/Si3N4/Al2O3/TiN structures. Appl Phys Lett 108:212103
Wang SY, Huang CW, Lee DY, Tseng TY, Chang TC (2010) Multilevel resistive switching in Ti/CuxO/Pt memory devices. J Appl Phys 108:114110
Wong HSP, Lee HY, Yu S, Chen YS, Wu Y, Chen PS et al (2012) Metal-oxide RRAM. Proc IEEE 100:1951
Prakash A, Jana D, Maikap S (2013) TaOx-based resistive switching memories: prospective and challenges. Nanoscale Res Lett 8:418
Long S, Zhang ZP, Wu Y, Wong HSP, Wong SS (2013) Nanometer-scale HfOx RRAM. IEEE Electron Device Lett 34:1005–1007
Long S, Lian X, Cagli C, Cartoixà X, Rurali R, Miranda E et al (2013) Quantum-size effects in hafnium-oxide resistive switching. Appl Phys Lett 102:183505
Kim S, Jung S, Kim MH, Kim TH, Bang S, Cho S, Park B (2017) Nano-cone resistive memory for ultralow power operation. Nanotechnology 28:125207
Wang IT, Lin YC, Wang YF, Hsu CW, Hou TH (2014) 3D synaptic architecture with ultralow sub-10 fJ energy per spike for neuromorphic computation. In: Proceedings of the IEEE International Electron Devices Meeting (IEDM), December (pp. 28–5). https://ieeexplore.ieee.org/abstract/document/7047127/?reload=true
Zhang L, Cosemans S, Wouters DJ, Govoreanu B, Groeseneken G, Jurczak M (2013) Analysis of vertical cross-point resistive memory (VRRAM) for 3D RRAM design. Int Memory Workshop:1–4. https://doi.org/10.1109/IMW.2013.6582122
Chen HY, Yu S, Gao B, Huang P, Kang J, Wong HSP (2012) HfOx based vertical resistive random access memory for cost-effective 3D cross-point architecture without cell selector. Int Electron Devices Meet 20(7):1–20.7.4. https://doi.org/10.1109/IEDM.2012.6479083
Lin YD, Chen YS, Tsai KH, Chen PS, Huang YC, Lin SH, Gu PY, Chen WS, Chen PS, Lee HY, Rahaman SZ, Hsu CH, Chen FT, Ku TK (2015) Highly robust self-compliant and nonlinear TaOx/HfOx RRAM for 3D vertical structure in 1TnR architecture. Intl Symp VLSI Tech Sys and App. https://doi.org/10.1109/VLSI-TSA.2015.7117559
Wang I-T, Chang C-C, Chiu L-W, Chou T, Hou T-H (2016) 3D Ta/TaOx/TiO2/Ti synaptic array and linearity tuning of weight update for hardware neural network applications. Nanotechnology 27:365204
Linn E, Rosezin R, Kugeler C, Waser R (2010) Complementary resistive switches for passive nanocrossbar memories. Nat Mater 9:403
Kim HD, Yun MJ, Kim S (2015) Self-rectifying resistive switching behavior observed in Si3N4-based resistive random access memory devices. J Alloy Compd 651:340–343
Wang Z, Kang J, Yu Z, Fang Y, Ling Y, Cai Y, Huang R, Wang Y (2017) Modulation of nonlinear resistive switching behavior of a TaOx-based resistive device through interface engineering. Nanotechnology 28:055204
Baek SJ, Lim KS (2010) Bipolar resistance switching driven by tunnel barrier modulation in TiOx/AlOx bilayered structure. Appl Phys Lett 97:072109
Shih C, Wang TH, Huang JS, Lai CC, Hong YJ, Chueh YL (2016) Roles of oxygen and nitrogen in control of nonlinear resistive behaviors via filamentary and homogeneous switching in oxynitride thin film memristor. RSC Adv 6:61221–61227
Chand U, Huang KC, Huang CY, Tseng TY (2016) Mechanism of nonlinear switching in HfO 2-based crossbar RRAM with inserting large bandgap tunneling barrier layer. IEEE Trans Electron Devices 62:3665–3670
Kim S, Park BG (2016) Tuning tunnel barrier in Si3N4-based resistive memory embedding SiO2 for low-power and high-density cross-point array applications. J Alloy Compd 663:419–423
Huang P, Chen S, Zhao Y, Chen B, Gao B, Liu L, Chen Y, Zhang Z, Bu W, Wu H, Liu X, Kang J (2016) Self-selection RRAM cell with sub-μA switching current and robust reliability fabricated by high-K/metal gate CMOS compatible technology. IEEE Electron Device Lett 63:4295–4301
Wang Z, Rao M, Midya R, Joshi S, Jiang H, Lin P et al (2017) Threshold switching of Ag or Cu in dielectrics: materials, mechanism, and applications. Adv Funct Mater 28:1704862
Ahn SE, Kang BS, Kim KH, Lee MJ, Lee CB, Stefanovich G, Kim CJ, Park Y (2009) Stackable All-Oxide-Based Nonvolatile Memory WithAl2O3Antifuse andp-CuOx/n-InZnOxDiode. IEEE Electron Devices Lett 30:550–552.
Huang JJ, Tseng YM, Hsu CW, Hou TH (2011) Bipolar NonlinearNi/TiO2/NiSelector for 1S1R Crossbar Array Applications. IEEE Electron Dev Lett 32:1427–1429.
Ielmini D (2008) Threshold switching mechanism by high-field energy gain in the hopping transport of chalcogenide glasses. Phys Rev B 78:035308
Chekol SA, Yoo J, Park J, Song J, Sung C, Hwang H (2018) A C–Te-based binary OTS device exhibiting excellent performance and high thermal stability for selector application. Nanotechnology 29:345202
Liu X, Sadaf SM, Son M, Shin J, Park J, Lee J, Park S, Hwang H (2011) Diode-less bilayer oxide (WOx–NbOx) device for cross-point resistive memory applications. Nanotechnology 22:475702
Lin CY, Chen PH, Chang TC, Chang KC, Zhang SD, Tsai TM, Pan CH, Chen MC, Su YT, Tseng YT, Chang YF, Chen YC, Huang HC, Sze SM (2017) Attaining resistive switching characteristics and selector properties by varying forming polarities in a single HfO2-based RRAM device with a vanadium electrode. Nanoscale 9:8586–8590
Hota MK, Nagaraju DH, Hedhili MN, Alshareef HN (2015) Electroforming free resistive switching memory in two-dimensional VOx nanosheets. Appl Phys Lett 107:163106
Wonga FJ, Sriram TS, Smith BR, Ramanathan S (2013) Bipolar resistive switching in room temperature grown disordered vanadium oxide thin-film devices. Solid State Electron 87:21–26
Xia M, Zhang K, Yang R, Wang F, Zhang Z, Wu S (2017) Electronic bipolar resistive switching behavior in Ni/VOx/Al device. Mater Sci Eng. B 221:35–40.
Liu CY, Sung PW (2011) Different resistive switching characteristics of a cu/SiO2/Pt structure. Jpn J Appl Phys 50:091101
You BK, Park WI, Kim JM, Park KI, Seo HK, Lee JY, Jung YS, Lee KJ (2014) Reliable control of filament formation in resistive memories by self-assembled nanoinsulators derived from a block copolymer. ACS Nano 8:9492–9502
Bricalli A, Ambrosi E, Laudato M, Maestro M, Rodriguez R, Ielmini D (2018) Resistive switching device technology based on silicon oxide for improved ON–OFF ratio—part I: memory devices. IEEE Trans Electron Dev 65:115–121
Yao J, Sun Z, Zhong L, Natelson D, Tour JM (2010) Resistive switches and memories from silicon oxide. Nano Lett 10:4105–4110
Chang YF, Chen PY, Chen YT, Xue F, Wang Y, Zhou F, Fowler B, Lee JC (2012) Study of polarity effect in SiOx-based resistive switching memory. Appl Phys Lett 101:052111
Chang YF, Fowler B, Chen YC, Chen YT, Wang Y, Xue F, Zhou F, Lee JC (2014) Intrinsic SiOx-based unipolar resistive switching memory. I. Oxide stoichiometry effects on reversible switching and program window optimization. J Appl Phys 116:043708
Wang Y, Qian X, Chen K, Fang Z, Li W, Xu J (2013) Resistive switching mechanism in silicon highly rich SiOx (x < 0.75) films based on silicon dangling bonds percolation model. Appl Phys Lett 102:042101
Fowler BW, Chang YF, Zhou F, Wang Y, Chen PY, Xue F, Chen YT, Bringhurst B, Pozderc S, Lee JC (2015) Electroforming and resistive switching in silicon dioxide resistive memory devices. RSC Adv 5:21215–215236
Mehonic A, Cueff S, Wojdak M, Hudziak S, Labbé C, Rizk R, Kenyon AJ (2012) Electrically tailored resistance switching in silicon oxide. Nanotechnology 23:455201
Yan X, Zhou Z, Ding B, Zhao J, Zhang Y (2017) Superior resistive switching memory and biological synapse properties based on a simple TiN/SiO2/p-Si tunneling junction structure. J Mater Chem C 5:2259
Mehonic A, Cueff S, Wojdak M, Hudziak S, Jambois O, Labbé C, Garrido B, Rizk R, Kenyon AJ (2012) Resistive switching in silicon suboxide films. J Appl Phys 111:074507
Chen YS, Lee HY, Chen PS, Chen WS, Tsai KH, Gu PY et al (2014) Novel defects-trapping TaOX/HfOX RRAM with reliable self-compliance, high nonlinearity, and ultra-low current. IEEE Electron Dev Lett 35:202–204
Wu Y, Lee B, Wong HSP (2010) Al2O3-based RRAM using atomic layer deposition (ALD) with 1-μA RESET current. IEEE Electron Dev Lett 31:1449–1451
Yang Y, Choi S, Lu W (2013) Oxide heterostructure resistive memory. Nano Lett 13:2908–2915
This work was supported by a grant from the National Research Foundation of Korea (NRF), funded by the Korean government (MSIP) (2018R1A2A1A05023517).
Availability of Data and Materials
All data and material are available.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Kim, S., Lin, C., Kim, M. et al. Dual Functions of V/SiOx/AlOy/p++Si Device as Selector and Memory. Nanoscale Res Lett 13, 252 (2018) doi:10.1186/s11671-018-2660-9
- Resistive switching
- Silicon oxide